Full Paper Fabrication, morphology and structural characterization of tungsten oxide nanorods T.Maiyalagan, B.Viswanathan* National Center for Catalysis Research, Department of Chemistry, Indian Institute of Technology Madras, Chennai 600 036, (INDIA) Phone : +91-044-22574200 ; Fax: +91-44-22574202 E-mail : email@example.com st Received: 1 September, 2007 ; Accepted: 6th September, 2007
ABSTRACT The Template synthesis of Tungsten oxide nanorods by calcination of Phosphotungtstic acid (HPW) on alumina membrane template is described. The nanorods were characterized by electron microscopic analyses, Raman, IR and X-ray diffraction techniques. SEM, TEM and AFM images reveal the hollow structures and vertically aligned features of the nanotubes and the phase structure of the WO3 was proved by X-ray diffraction. In addition, it is observed that the cycle ability of the nanorods is superior to that of bulk materials, which implies that the morphology has an influence on the electrochemical performances of the material. ďƒ“ 2007 Trade Science Inc. - INDIA
KEYWORDS Tungsten oxide nanorods; Template synthesis; Alumina template.
The rich structural chemistry of tungsten oxides encompasses a multitude of interesting compounds and a wide There is great interest in the synthesis of one-di- spectrum of tungstic acids and different WO3 phases. mensional nanostructured materials because of its po- Tungsten oxide is an important functional material. In tential applications in many areas. Metal-oxide semi- recent years, a variety of nanometer-scaled structures conductors such as WO3, TiO2, and ZnO and SnO2 of tungsten oxide have been developed. These nano are widely used in sensors, having high detection ability structures have demonstrated promising properties. To and stability[1â€“3]. These transition metal oxides have date, WO3 has been one of the most extensively studdrawn much attention from scientists in recent years ied materials for its Electrochromic, photochromic and because they are applied as electrochromic materials. thermo chromic properties for use in devices, such as Their potential applications include several technologi- information displays, sensor devices and smart Wincal areas. Tungsten metal, tungsten oxides and tung- dows. In addition, WO3 has a high potential for use in states represent a fascinating class of materials. Tung- electrochemical devices, such as rechargeable lithium sten wires/filaments are widely used as tips for field batteries, owing to its rich chemical intercalation reacemission and tips for scanning tunneling microscopy. tivity. The oxides of transition metal tungsten have at-
Tungsten oxide . nanorods
Full Paper tracted constant research interest for the past few decades due to their wide applicability as gas sensors for SO2 and H2S[5,6], as excellent field emitters(specifically W18O49) and as photo anodes in photochemical cells. In addition, WOx have also found unique application in electro chromic devices due to their excellent voltage-modulated optical properties. Tungsten oxide(WO3) is an n-type semiconductor with a reported band gap of about 2.6-2.8eV. The intrinsic conductivity arises from its non-stoichiometric compositiongiving rise to a donor level formed by oxygen vacancy defect in the lattice. Since tungsten has many oxidation states, i.e., 2, 3, 4, 5 and 6, the tungsten compound can exist in many forms. For instance, the typical forms of tungsten oxides are tungsten(VI) oxide(WO3, lemon yellow appearance) and tungsten(IV) oxide(WO2, brown and blue appearance). Such electronic properties make the tungsten oxides suitable for various applications such as electrochromic, photochromic, photocatalyst, and gas sensors[15-17]. Various methods including chemical vapour deposition, electrochemical deposition, laser vaporization[20, 21] have been used to prepare tungsten oxide thin films. In conventional WO3 thin films with nanoscale-sized grains, the electrical conduction is mainly controlled by free carrier transport across the grain boundaries. So the synthesis of mono crystalline tungsten oxide as nano wires or nanorods is of great interest. In the past years, Zhu et al. produced a micrometer scale tree-like structure by heating a tungsten foil, partly covered by SiO2 in Ar atmosphere at 16000C. These nanostructures were composed by monoclinic W18O49 nanoneedles and WO3 nanoparticles. Nanorods of several oxides including WO3 have been prepared by templating on acid-treated carbon nanotubes. By heating WS2 in oxygen, fibers of W18O49 were produced with a pine-treelike structure. Mixtures of WO2 and WO3 with nanorods structure were obtained by Koltypin et al. via amorphous tungsten oxide nanoparticles. Li et al. have synthesized WO3 nanobelts and nanorods via physical vapour deposition process where the nanostructures were deposited on silicium wafers maintained at 6000C. Recently Liu et al. reported on the preparation of tungsten oxide nanowires through a vapour-solid growth process by heating a tungsten wire partially wrapped with boron oxide at 12000C and Shingaya et al. pre-
pared by oxidation at high temperature well-oriented WOx nanorods on a(0. 01)W surface. However, the study on nanoscaled WO3 materials is still in its infancy due to lack of suitable preparation method. In the present work, we report a novel route for template synthesis of crystalline WO3 nanorods. Our work on the tungsten oxide tubular structures featured a low cost and an easy manipulation technique. In the fabrication, no catalyst was involved and only a rough vacuum was required. EXPERIMENTAL Materials All the chemicals used were of analytical grade. Phosphotungstic acid(Sisco Research Laboratories, India), dichloromethane and concentrated HF(Merck) were used. Alumina template membranes were obtained from Whatman Anopore Filters. Anodisc alumina membranes with a pore size of 200nm and thickness of 60ď m were purchased from Whatman(catalog no. 68096022; Maidstone, U.K.). Synthesis of Tungsten oxide nanorods. 10g of Phosphotungtstic acid(H3PW12O40) was stirred in a 30ml of methanol solution. The resulting colloidal suspension was infiltrated into the membrane under vacuum by wetting method. The same procedure was repeated 1 to 8 times. The upper surface of the membrane was then polished gently by sand paper(2500 grit) and dried at 368 K for 1 h. The formation of WO3 nanorods inside alumina template(WO3 / AAO) was further achieved by programmed temperature thermal decomposition from 95 to 5000C min-1 and finally calcinated at 873K for 3h in air. The removal of the AAO template was performed by dissolving alumina template in 10%(v/v) HF. The WO3 nanorod product was washed with a copious amount of deionized water, to remove the residual HF and dried at 393 K. Characterization methods The scanning electron micrographs were obtained after the removal of alumina template using a JEOL JSM-840 model, working at 15keV. For transmission electron microscopic studies, the nanorods dispersed in ethanol were placed on the copper grid and the im-
T.Maiyalagan and B.Viswanathan
Full Paper temperature with 514.5nm excitation in backscattered mode using Bruker FRA106 FT-Raman instrument. The IR spectrum was recorded with Perkin-Elmer (L-710) spectrophotometer. Electrochemical measurements
Figure 1 : (a) SEM Micrograph of the WO3 nanorod and (b) AFM micrograph of the nanorod
The catalyst was electrochemically characterized by cyclic voltammetry(CV) using an electrochemical analyzer(Bioanalytical Sciences, BAS 100). A common three-electrode electrochemical cell was used for the measurements. The counter and reference electrodes were a platinum plate(5cm2) and a saturated Ag/AgCl electrode respectively. The CV experiments were performed using 1M H2SO4 solution at a scan rate of 50 mV/s. All the solutions were prepared by using ultra pure water (Millipore, 18M). The electrolytes were degassed with nitrogen before carrying out the electrochemical measurements. Preparation of working electrode
Figure 2 : (a) TEM Micrograph of the WO3 nanorod and (b) EDS pattern of nanorod
Wave number(cm -1 )
Figure 3 : FT-IR Spectrum of the (a) Calcined HPW (b) Bulk WO3 and (c) WO3 nanorods
Glassy carbon (GC) (BAS Electrode, 0.07cm2) was polished to a mirror finish with 0.05m alumina suspensions before each experiment and this served as an underlying substrate of the working electrode. In order to prepare the composite electrode, the nanorods were dispersed ultrasonically in water at a concentration of 1mg ml-1 and 20l aliquot was transferred on to a polished glassy carbon substrate. After the evaporation of water, the resulting thin catalyst film was covered with 5-wt% Nafion solution. Then the electrode was dried at 353 K and used as the working electrode. RESULTS AND DISCUSSION
The morphology of tungsten oxide nanorods was ages were obtained using Phillips 420 model, operating studied with SEM, AFM, transmission electron microsat 120keV. The nanorods were sonicated in acetone copy (TEM) images on a Philips CM12/STEM instrufor 20 minutes and then dropped on cleaned Si sub- ment. The scanning electron microscopy (SEM) image strates. Next the AFM imaging was performed in air presented in figure 1(a) shows the rod like morphology using a Nanoscope IIIA atomic force microscope (Digi- of the product. Further the AFM image confirms the tal Instruments, St. Barbara, CA) operated in contact rod like morphology in figure 1(b) which represents low mode. magnification. The morphology of the nanorods can be The X-ray diffraction patterns were obtained on a confirmed with TEM micrograph shown in figure 2(a). Philips PW1820 diffractometer with CuKá (1.54178 Å) The dimensions of the nanorods were matched with the radiation. The WO3 nanorods placed in glass capillary outer diameter of the template used. The diameter of tubes were used for recording Raman spectrum at room the nanorods was found to be around 200nm.
Tungsten oxide . nanorods
Potential(V) Raman shift (cm-1 )
Figure 4 : Raman spectrum of the WO3 nanorods
Figure 6 : Cyclic voltammograms for (a) Bulk WO3 and (b) WO3 nanorods in 1M H2SO4 at scan rate of 50mV s-1 at 298K 20(degrees)
813cm-1 correspond to the stretching modes of the WO3[30-32]. The XRD pattern for the as-synthesized The composition of the nanorods was investigated tungsten oxide nanorods and Phosphotungstic acid are using an energy dispersion spectroscopy (EDS). Figure given in figure 5(a,b) respectively. The diffraction peaks 2(b) shows EDS of the WO3 nanorods. EDS analysis and the peak intensities of the tungsten oxide nanorods indicates that the nanorods are mainly composed of W are in good agreement with the diffraction peaks of crysand O (the Cu signal comes from the TEM grids). No talline monoclinic phase of WO [33,34]. 3 evidence of impurities was detected in the WO3 nanorods. The electrochemical behavior of bulk WO3 and The FT-IR spectra of WO3 nanorods recorded in WO nanorods were studied in 1M H SO as shown in 3 2 4 the region 400-3500cm-1 are shown in figure 3. The figure 6. The cyclic voltammogram shows an anodic broad band from 1000cm-1 to 500cm-1 corresponds to peak current at -0.07V and it is due to the formation of the W-O vibrational mode. It has been widely reported tungsten bronzes by hydrogen intercalation in the tungthat HPW with Keggin structures gives several strong, sten trioxide. The electrochemical response due to W typical IR bands at ca. 1079cm-1(stretching frequency is seen at -0.1V in the forward scan, which matches of P-O of the central PO4 tetrahedron), 983cm-1(ter- with the peak reported in literature. Further, the staminal bands for W=O in the exterior WO6 octahedron), bility of tungsten trioxides in sulphuric acid medium was 889 cm-1 and 805 cm-1(bands for the W-Ob-W and W- evaluated by carrying out the cyclic voltammetry by Oc-W bridge, respectively). repeating voltammetric cycles in 1M H2SO4. An initial The raman spectra of WO3 nanorods exhibiting decrease in current was observed and after few cycles bands at ď ž717 and 808cm-1 are shown in figure 4. These the peak current remained the same even after 50 cycles bands agree closely to the wave numbers of the stron- and this confrims the stability of WO nanorods in sul3 gest modes of monoclinic-WO3. The bands at 703 and furic acid medium. Figure 5 : XRD patterns of (a) HPW and (b) WO3 nanorods
T.Maiyalagan and B.Viswanathan
Full Paper CONCLUSIONS In summary, a simple template synthesis method has been described for preparing WO3 nanorods by a direct calcination of Phosphotungtstic acid(HPW) in the channels of the alumina template. The size of nanorods is around 200nm which matches with the diameter of the template used. The Tungsten oxide nanorods with controlled morphology and composition have been achieved. The morphology of the aligned nanostructures was verified by SEM, AFM and TEM. It was found that WO3 nanorods exhibit higher electrochemical activity and stability compared to bulk WO3. REFERENCES  P.Heszler, L.F.Reyes, A.Hoel, L.Landstrom, V. Lantto, C.G.Granqvist; Proc.Soc.Photo-Opt.Instrum. Eng., 5055, 106 (2003).  M.J.Madou, S.R.Morrison; Chemical Sensing with Solid State Devices, (1989).  G.Sberveglieri (Ed.); Gas Sensors, Kluwer, Dordrecht, The Netherlands, (1992).  Z.Liu, Y.Bando, C.Tang: Chem.Phys.Lett., 372, 179 (2003).  M.Stankova, X.Vilanova, J.Calderer, E.Llobet, P.Ivanov, I.Gracia, C.Cane, X.Correig; Sens. Actuators, B102, 219 (2004).  J.L.Solis, S.Saukko, L.Kish, C.G.Granqvist, V. Lantto; Thin Solid Films, 391, 255 (2001).  Y.Li, Y.Bando, D.Golberg; Adv.Mater., 15, 1294 (2003).  C.Santato, M.Odziemkowski, M.Ulmann, J. Augustynski; J.Am.Chem.Soc., 123, 10639 (2001).  C.G.Granqvist, E.Avendano, A.Azens; Thin Solid Films, 442, 201 (2003).  M.A.Butler; J.Appl.Phys., 48, 1914 (1977).  Solid state structure of tungsten trioxide. Available online at http://www.webelements.com.  C.G.Granqvist; Solar Ener.Mater., 60, 201 (2000).  M.Sun, N.Xu, Y.W.Cao, J.N.Yao, E.G.Wang; J. Mater.Res., 15, 927 (2000).
 G.R.Bamwenda, H.Arakawa; Appl.Catal., A210, 181 (2001).  M.Akiyama, J.Tamaki, N.Miura, N.Yamazoe; Chem.Lett., 16, 11 (1991).  A.A.Tomchenko, V.V.Khatko, I.Emelianov; Sens. Actuators, B46, 8 (1998).  D.S.Lee, S.D.Han, J.S.Hun, D.D.Lee; Sens. Actuators, B60, 57 (1999).  E.Brescacin, M.Basato, E.Tondello; Chem.Mater., 11, 314 (1999).  Z.R.Yu, X.D.Jia, J.H.Du, J.Y.Zhang; Sol.Energy Mater.Sol.Cells, 64 55 (2000).  M.Sun, N.Xu, J.W.Yao, E.C.Wang; J.Mater.Res., 15, 927 (2000).  S.T.Li, M.S.El-Shall; Nanostruct.Mater., 12, 215 (1999).  Y.Q.Zhu, W.Hu, W.K.Hsu, M.Terrones, N.Grobert, J.P.Hare, H.W.Kroto, D.R.M.Walton, H.Terrones; Chem.Phys.Lett., 309, 327 (1999).  B.C.Satishkumar, A.Govindaraj, M.Nath, C.N.R. Rao; J.Mater.Chem., 10, 2115 (2000).  W.B.Hu, Y.Q.Zhu, W.K.Hsu, B.H.Chang, M. Terrones, N.Grobert, H.Terrones, J.P.Hare, H.W. Kroto, D.R.M.Walton; Appl.Phys.A., 70, 231 (2000).  Y.Koltypin, S.I.Nikitenko, A.Gedanken; J.Mater. Chem., 12, 1107 (2002).  Y.B.Li, Y.Bando, D.Golberg, K.Kurashina; Chem. Phys.Lett., 367, 214 (2003).  Z.Liu, Y.Bando, C.Tang; Chem.Phys.Lett., 372, 179 (2003).  R.S.Wagner, W.C.Ellis; Trans.Met.Soc.AIME, 233, 1053 (1965).  C.Santato, M.Odziemkowski, M.Ulmann, J. Augustynski; J.Am.Chem.Soc., 123, 10639 (2005).  M.Figlarz; Prog.Solid-State Chem., 19,1 (1989).  M.F.Daniel, B.Desbat, J.C.Lassegues, B.Gerand, M.Figlarz; J.Solid State Chem.67(2), 235 (1987).  S.H.Lee, H.M.Cheong, C.E.Tracy, A.Mascarenhaus, D.K.Benson, S.K.Deb; Electrochim.Acta 44, 3111 (1999).  O.Yamaguchi, D.Tomihisa, H.Kawabata, K.Shimizu; J.Am.Ceram.Soc.70, 94 (1987).  P.M.Woodward, A.W.Sleight; J.Solid State Chem. 131, 9 (1997).